**Dangling-bond defect in a-Si:H: Characterization of network and strain effects**

**by first-principles calculation of the EPR parameters**

G. Pfanner, C. Freysoldt, and J. Neugebauer

*Max-Planck-Institut f¨ur Eisenforschung GmbH, D-40237 D¨usseldorf, Germany*

F. Inam and D. Drabold

*Department of Physics and Astronomy, Ohio University, Athens, Ohio 45701, USA*

K. Jarolimek*_{and M. Zeman}

*PVMD/DIMES, Delft University of Technology, 2600 GA Delft, The Netherlands*
(Received 19 December 2012; published 12 March 2013)

The performance of hydrogenated amorphous silicon (a-Si:H) solar cells is severely affected by the
light-induced formation of metastable defects in the material (Staebler-Wronski effect). The common notion is that the
dangling-bond (db) defect, a threefold coordinated silicon atom, plays a key role in the underlying mechanisms.
To support the characterization of this defect by electron paramagnetic resonance (EPR), we present in this work
a first-principles study of the EPR parameters for a structural ensemble of the db defect. We show that the a-Si:H
dangling bond is a network defect for which charge and spin localization substantially depend on the actual
coordination of the db atom and the local geometric and electronic structure of the immediate surrounding. It
consequently differs by its very nature from its crystalline counterpart, which is typically related to the presence
of a vacancy. The application of hydrostatic strain to our models yields further insights into the dependence of
the hyperfine interaction on the structural characteristics of the defect. The observed trends are shown to result
*from the interplay between delocalization and sp hybridization.*

DOI:10.1103/PhysRevB.87.125308 *PACS number(s): 71.15.Mb, 71.55.Jv, 76.30.−v*

**I. INTRODUCTION**

Thin-film amorphous silicon (a-Si:H) is an established
material for flexible, low-cost, and nontoxic solar cells.
How-ever, the major drawbacks of a-Si:H solar cells are their low
*conversion efficiency η and—related to that—the degradation*
over time due to light exposure—the Staebler-Wronski effect1

(SWE). Due to the SWE, a single-junction solar cell loses about 30% of its initial efficiency after 1000 h of illumination.2

The SWE is metastable and annealing at 100–250◦C restores
the conversion efficiency within a few minutes.3Similarly, one
observes seasonal fluctuations in real-life a-Si:H solar cells,
*with a partial recovery of η in the summer months.*4

The SWE is related to structural changes in the material,
i.e., the formation of metastable defects. However, a full
understanding of the relevant processes has not been obtained
so far. One of the reasons is that the notion of a structural defect
is conceptually complicated in the amorphous phase. Initially,
it is only characterized by the corresponding deviation from
*the ideal nearest-neighbor coordination N*= 4 (see Fig. 1).
However, the complex local structure often makes a clear
distinction between different kinds of defects (e.g., dangling
bond, broken bond, floating bond) difficult. Commonly, the
SWE is believed to be related to the creation of a dangling
bond (db), i.e., a threefold coordinated silicon atom with the
remaining electron being unpaired and strongly localized.5–7
But there is no consensus on the specific defect-creation
mechanism. Several models have been suggested over the
years as reviewed elsewhere.8,9 _{Besides the db defect, there}

are indications that strained regions contribute to the Staebler-Wronski effect as well.8,10–12

Atomistic-scale information about the defect is crucial for a better understanding of the Staebler-Wronski effect.

Experimentally this can be obtained by electron paramagnetic
resonance (EPR), which probes for the local atomic structure
of defects with unpaired spins,13_{such as the silicon dangling}

bond. In the case of a-Si:H, the resulting absorption spectrum
is mainly characterized by the interaction of the unpaired
*spin with the external magnetic field (Zeeman interaction, g*
tensor) and with the nuclear dipole moment of the defect atom
*(hyperfine interaction, A tensor). However, structural disorder*
of the material leads to a broad spectral distribution,5–7,14
which cannot be assigned to a specific defect structure. Further
insights into the relevant features can only be obtained by
com-paring experimental results with theoretical calculations.14–19

Simple molecular db systems such as the tetrasilyl-radical
(SiH3)3Si• are able to capture the experimental notion of a
strongly localized defect wave function.5–7_{Both EPR tensors}

* (g and A) are uniaxial, which means that there is a rotational*
symmetry (at least threefold) about a unique axis.13

_{The}

hyperfine interaction is directly connected to the local defect
geometry.17,19 _{For example, the variation of the }

dangling-bond dangling-bond angle (to its backdangling-bond neighbors) yields trends
in the hyperfine parameters, which can be reasoned by the
*s- and p-like character of the db orbital. In the crystalline*
(c-Si) environment, dangling bonds are created from
vacancy-impurity complexes19–22 _{or hydrogen complexes in }

vacan-cies, at surfaces,19–21,23 _{and at interfaces.}24–26 _{The structural}

network of these systems can be crucial for the hyperfine
*interaction, which overall reflects the interplay between sp*
hybridization of the db orbital and spin delocalization.19

In this work we present a first-principles study of the EPR parameters of the dangling bond in a-Si:H. By this approach we are able to characterize the local defect structure and the effect of the network. Most notably, we find that the latter exerts a

FIG. 1. (Color online) Random-network model of a-Si:H illus-trating various local structural characteristics. The colors indicate coordination [white: 1 (hydrogen), red: threefold (dangling bond), blue: fourfold, green: fivefold (floating bond)]. In this work we use periodic-boundary conditions and a supercell approach for the modeling of the amorphous structure.

much more important influence than in the crystalline matrix.
We then apply hydrostatic strain to our a-Si:H db models to
gain insights into their structural stability, which is required
for elaborating the differences to other kinds of possible defect
mechanisms such as strained regions.8,10–12_{This study reveals}

the different nature of the c-Si and a-Si:H dangling bond, and can also in part explain the remaining discrepancies between theoretical and experimental findings.

**II. COMPUTATIONAL METHODS**

In this work we employ periodic-boundary conditions and a
supercell-based approach. For the creation of the db models we
start from defect-free a-Si:H models, which were either created
by releasing hydrogen into Wooten-Winer-Weaire models
of a-Si,27 _{or by heating and gradually annealing of c-Si:H}

models followed by structural relaxation.28,29 The dangling
bond is then created by removing one hydrogen atom from the
supercell with a subsequent relaxation of the atoms. We note
in passing that in some cases the network rearranges so that the
dangling bond moves away from the site where the hydrogen
atom has been taken out. For our investigation we use 26
small (64Si-7H) as well as 28 large db models (216Si-29H).
The generation of the structures as well as the computation
*of the EPR parameters (most notably, the g tensor) is*
resource demanding, and we can therefore only simulate a
subensemble of realistically occurring defect configurations
(1015–1019 *defects/cm*3 in experiment30). Second, the ratio
between silicon and hydrogen atoms yields a hydrogen
concentration on the order of 11–13%. Experimentally it can
have a much larger fluctuation on the order of 7–30%.7,14

*For the ab initio calculation of the EPR parameters, we*
have used the plane-wave DFT codeQUANTUM ESPRESSO31
(v4.2.1), in which the GIPAW formalism32 has been
re-cently implemented. We employ the Perdew-Burke-Ernzerhof
functional33 _{and norm-conserving pseudopotentials}34 _{with a}

scalar-relativistic correction for silicon.35,36 _{We use the same}

**plane-wave cutoff (30 Ry), and k-point mesh**37_{(6}_{× 6 × 6 for}

the small supercells and 4× 4 × 4 for the large supercells) as

established in a previous work on c-Si db models.21_{Here also}

a good agreement between theory and experiment was found,
*specifically the deviation for the g tensor is on the order of a*
few 10−3and up to 3% for the hyperfine parameters. Thus our
approach is able to accurately characterize the defect structure
of localized dangling bonds in silicon.

Experimentally, only the absolute value of the hyperfine couplings can be determined from powder spectra. In our calculations we keep the negative sign due to the negative gyromagnetic ratio of silicon, but follow the experimental notion that the magnitude of the coupling is determined by the absolute value.

To study the effect of hydrostatic strain we change the lattice constant of the model, and then relax the atomic positions within the cell. We only consider the smaller 64Si-7H supercells. However, we do not expect drastic differences for the larger supercells, because the EPR-parameter statistics of both are quite similar, which agrees well with previous findings for other key properties such as the radial distribution function, the band gap, and tail states.28,29

**III. RESULTS AND DISCUSSION**
**A. EPR parameters of the whole ensemble**

The most natural assumption is that the described
genera-tion of the models indeed creates a dangling bond in the
amor-phous matrix, even though network rearrangements occurring
during relaxation may strongly modify the character of the
defect. The statistical average of our models should therefore
correspond to a metastable dangling bond at a random position
in the a-Si:H network. From this unbiased approach, previous
studies draw the following conclusions.14,38*The theoretical g*
tensor has rhombic symmetry and it is in good agreement
*with experimental results. The A tensor is axial, and the*
experimentally observed redshift of the isotropic contribution
*a* *from the crystalline (a*c-Si∼ −300 MHz) to the a-Si:H
*matrix (a*_{a-Si:H}exp ∼ −200 MHz) can only be reproduced by our
calculations in part with a remaining discrepancy on the order
of 70 MHz. This indicates a selection of dangling bonds in
experiments, which needs to be clarified by complementary
*studies of possible mechanisms. The g and A tensor have*
*different symmetry properties since the g tensor reflects*
*the global electronic defect structure, while the A tensor is*
exclusively determined by the local spin-density distribution
in the vicinity of the nucleus of interest. Consequently, in
*some cases one obtains similar g values for models with a*
quite different degree of spin localization. This implies that
*the g tensor holds little information about the local defect*
geometry, and we will therefore put our focus on the hyperfine
interaction in the following.

**B. Classification by coordination and spin localization**
Going beyond the statistical picture, one has to establish
criteria according to which one can classify the a-Si:H
db models. We regard the atom with the largest hyperfine
interaction as the central atom of the defect, i.e., the db atom.
First, it is necessary to check for the coordination at this atom,
i.e., that it is indeed bonded to exactly three defect neighbors.
To investigate this question, we consider two parameters,

*the number of atoms within a certain distance rcut* and the
bonding to hydrogen. We find that 43 models (80%) are triply
coordinated for the reasonable cut-off bond length of 2.42 ˚A,
and only four models (7%) do have a hydrogen as a backbond
neighbor. Within our limited ensemble it is therefore more
likely that the dangling bond has only silicon neighbors in
accordance with recent experimental studies.39,40

Another important aspect is the degree of spin localization,
which we quantify by looking at the largest and second largest
*a*_{2nd}*value for each db model. For crystalline models, the a*2nd
value is relatively constant at around−30 MHz, and it always
occurs at the second-nearest backbond neighbor.19,21,24In the
amorphous case, the situation is far more complex, and some
*models even have a2nd>*−100 MHz. Clearly in these cases
the spin is delocalized. In order to draw a line in between the
localized and delocalized db models, we chose that a model
*belonging to the former category must not have an a*2ndlarger
than−80 MHz. According to this criteria, 38 db models (70%)
are localized. A common feature of the delocalized models is
*that the a parameter at the dangling bond is usually smaller*
than*−250 MHz and the anisotropic b parameter*13_{is not larger}

than−30 MHz. This is again consistent with our picture of spin delocalization, which becomes apparently much more important in the amorphous environment.

**C. The characteristics of strongly localized dangling bonds**
As mentioned, the common notion of the amorphous db
defect is that it is indeed threefold coordinated and that
the spin is strongly localized on the central defect atom.
In the following we take this into account by applying the
mentioned criteria and only considering the subensemble of 33
models (61%) corresponding to a strongly localized, threefold
coordinated db defect either bond to three silicon atoms or
two silicon and one hydrogen atom. This procedure has also
the advantage that we can work out the structural differences
between the defect in the crystalline and the amorphous matrix.

**1. Bonding geometry at the db atom**

The bond lengths at the db atom are rather homogeneous
*with the mean value (standard deviation) l= 2.34(0.02) ˚A.*

The bond angles at the db atom are close to the tetrahedral angle
*but do have a large variation α= 109.7*◦*(12.6*◦). For reference,
the corresponding parameters for c-Si dangling bonds21 _{are}

*on average l= 2.35(0) ˚A and α = 110.7*◦*(1.9*◦). On the
other hand, a-Si:H models created by molecular dynamics28

*have on average the mean parameters l= 2.38(0.05) ˚A and*
*α= 108.9*◦*(13.6*◦), and experimentally one typically obtains
*a bond length of l= 2.35–2.37 ˚A and a standard deviation for*
*the angle distribution of 7.9*◦*–9.6*◦. Most notably, this means
that the theoretical angle distribution is larger than observed
in experiment.28_{For our purposes, it is important to stress that}

these values refer to an average over a whole structural model or over the results obtained from a sample. Overall we can see that the local defect geometry of the a-Si:H dangling bond does not vary substantially neither from their crystalline coun-terparts nor from the rest of the network, and that the structural disorder mostly originates from fluctuations in the bond angle.

**2. Hyperfine interaction**

The EPR parameters of the localized db models essentially
yield the same mean values compared to the overall ensemble,
*specifically the g values are shifted only by 0.0004 and*
*the hyperfine parameters by a∼ 10 MHz, b ∼ 7 MHz.*
Furthermore, the hyperfine parameters cannot be correlated
unambiguously to the local bond geometry since the variation
in between the smallest and the largest bond angle is typically
more than 10◦, and fluctuations of that order can have a drastic
effect.19 _{Indeed, a closer inspection reveals that there is no}

clear trend between the hyperfine and structural parameters.
* 3. Superhyperfine interaction and spin delocalization*
Despite the similar bond parameters, a-Si:H dangling bonds
have a smaller isotropic hyperfine coupling as their crystalline

*counterparts [(a∼ −60 MHz), (b ∼ −10 MHz)]. This*clearly indicates a stronger spin delocalization in the former case and can be understood by looking at the isotropic superhyperfine interaction of the silicon atoms. The most important difference is that the a-Si:H db models can also have strong isotropic couplings for atoms that are not second-nearest neighbors. This is illustrated in Fig. 2(a), which

5 0 5
80
70
60
50
40
30
20
10
*d*
*a*
MH
z
(a) (b)

FIG. 2. (Color online) (a) Example of a localized dangling bond with a strong isotropic hyperfine interaction on the first neighbor (in green).
*(b) The dependence of the isotropic hyperfine coupling a on the distance d from the db atom. We only consider significant couplings, chosen*
to be larger than−10 MHz, and we distinguish between opposite (positive parameter range) and backbond (negative parameter range) atoms.
Details of this classification scheme are described in the text.

shows a dangling bond with a significant spin density at the first backbond neighbor. To quantify the complexity of the spin distribution in the network, we depict in Fig.2(b)

the dependence of the isotropic superhyperfine coupling on
the distance from the db atom. In doing so, we apply a criteria
to distinguish between the backbond and the opposite db
side. First we compute the centroid of the triangle spanned
by the three nearest neighbors, the backbond atoms. Then
*we compare the distance ddb,n* *between an atom (with a >*
*10 MHz) and the db atom with the distance dc,n*between the
centroid and the atom. If the atom is closer to the centroid,
*dc,n< ddb,n, we consider it as on the backbond site, and as*
opposite otherwise. In the former case we assign a minus to
the distance, and in the latter case a plus, respectively. Overall
this gives us the following basic notion of the spatial spin
distribution in the supercell, which reflects the shell structure
of the network. As expected from the crystalline db models,
the strongest couplings occur around the second-nearest
neighbor distance, even though there is no difference between
opposite and backbond since for both cases the superhyperfine
interaction is similar in magnitude. This again indicates that
in our simulations dangling bonds appear rather randomly at
sites with an appropriate geometric distortion in the network
with a rather homogeneous distribution of neighbors. They
differ in this aspect from their crystalline counterparts, which
are typically related to the presence of a vacancy19,21 _{or an}

interface.24–26_{In this context it is reasonable but still interesting}

that the superhyperfine coupling is on average larger than in the crystalline environment. Apparently this is another manifestation of the delocalization, which is—as we have seen—a characteristic feature of a-Si:H dangling bonds.

For completeness, we mention that despite their small number, dangling bonds with a hydrogen at the backbond side have rather diverse EPR parameters with a distribution comparable to dangling bonds with only silicon backbond neighbors. From the overall isotropic couplings of hydrogen we see the same features as for neighboring silicon atoms. First, it is distributed homogeneously with respect to the distance from the db atom, which is in agreement with a recent experimental observation.39 Furthermore, hydrogen can have a significant spin polarization on the order of 30 MHz also for

larger distances (5 ˚A) from the db atom. This implies that the point-dipole approximation39does not allow for a quantitative analysis of distances.

We have seen that the amorphous host matrix gives rise to
a much broader spectrum of db-like defects than observed in
crystalline silicon. On the one hand, the removal of a hydrogen
atom from the system does not necessarily lead to the creation
of a strongly localized db defect as it is largely believed in
the literature.5–7_{Deviations from the threefold coordination as}

well as rather delocalized spin densities occur. Consequently, both aspects are characteristic for the a-Si:H dangling bond. The a-Si:H db is—in contrast to the vacancy-based c-Si db—a network defect, which most likely appears for suitable geometrical distortions with the local variation in the bond angle as the most important influence.

**D. Strain**

The different origins of the c-Si and the a-Si:H dangling
bond can also be illustrated by considering the effect of
hydrostatic strain on the hyperfine parameters. Of course,
a-Si:H films are typically biaxially strained.41 _{However, test}

calculations demonstrated the same trends as the computa-tionally more feasible study of hydrostatic strain. This can be explained intuitively by the more or less random orientation of the dangling bond in a-Si:H. In most cases, it is not aligned to any of the axes, and consequently it is not important, in which directions strain is applied.

The amorphous db models show a large structural
sensitiv-ity to strain. In particular for large strains (tensile or
compres-sive) one observes a redistribution of the spin density, and the
dangling bond hops from one to the other atom, which again
illustrates the network character of the defect. To take this into
account, we consider for each model only the range in which
the dangling bond is stable. Practically, this is implemented
by first determining the db atom at the ideal lattice constant.
Then we monitor whether it is still the atom with the largest
*a*value as a function of the applied strain. Furthermore, since
the bonding parameters of Si-H bonds cannot be compared
to Si-Si bonds, we only consider those cases in which the
dangling bond has three silicon atoms as neighbors.

0.06 0 0.05 0.1
2.3
2.4
2.5
2.6
2.7
*x x0* *x0*
bo
nd
le
ng
th
average
*V SiH* *3*
0.06 0 0.05 0.1
90
95
100
105
110
115
120
*x x0* *x0*
bo
nd
a
n
g
le
deg

*FIG. 3. (Color online) The dependence of bond length and bond angle on the elongation x from the ideal lattice constant x*0. For the

*rhombic supercells, x*0*corresponds to the mean lattice constant of the three axis (x*1*, x*2*, x*3). The bond parameters are defined by the average

over the three nearest neighbors. Each thin line corresponds to one db model. The thick blue line indicates the trend for the mean value. Kinks
in this curve can occur when the number of included db models changes with respect to strain. For comparison the thick dashed line shows the
*dependence of the crystalline V (SiH*3) db model. Values of pressure are included for the experimentally relevant range of strains.

First let us look at the structural parameters of the db atom
as depicted in Fig.3. For the mean bond length we recognize
that the amorphous db models show on average the same
*trends as the crystalline V (SiH*3) db model.42In particular, for
compressive strain they have a comparable range of stability,
*and besides that, the increase of l for tensile strain is on the*
same order. Significant deviations from this are only observed
*for l > 2.6 ˚*A when the model is not triply coordinated at the
ideal lattice constant. A similar correspondence is also found
*for the bond angle α in the case of tensile strain since the*
a-Si:H db models also favor a rather planar geometry. On the
other hand, the diverse picture for compressive strain can be
explained by inhomogeneities in the three bond angles which
are not captured by the mean parameter. To exemplify this
point let us look at the db model with the largest deviation from
*the overall trend (α= 109.6*◦*for x= 0.1). Even though the*
stability of the dangling bond is very sensitive to tensile strain,
it is threefold coordinated and localized at the ideal lattice
*constant, i.e., a true db model. The bond angles at x= x0*
vary by±5◦from the square angle, and for large tensile strain
*(x* *= 0.1) this tendency is enhanced since in this case α is in*
between 101 and 116 deg. The large variation among the three
bond angles illustrates that the mean value is indeed only an
approximative measure of an actually more complex bonding
geometry. Despite this deficiency, we learn from Fig. 3that
the bond parameters in general show the same trends as for
the crystalline db models, and that the bond angles are more
sensitive to compressive strain than the bond lengths.

The isotropic hyperfine interaction has no clear trend
(Fig. 4) since we are considering all db models (despite
their coordination and spin localization) on equal footing.
Consequently, it can happen that the spin density at the db
atom increases or decreases with applied strain, or that it
is rather delocalized over the whole range. In one case, the
*dangling bond is only stable in between x= [−0.004,0]*
before it starts to bond to hydrogen. On the other hand,
*the trend for the b parameter is rather homogeneous for*
almost all models and corresponds to the one observed for
the crystalline model with a constant shift of 20 MHz.
The only exceptions are caused by delocalization,
under-coordination, and a very small bond angle. However, the

true information here is obtained again from the averaged
*trends. The a parameter stays rather constantly in between*
200 and 250 MHz throughout the strain range, and there is no
obvious dependence on the magnitude of the applied strain.
This aspect distinguishes the a-Si:H dangling bonds from their
crystalline counterparts,19,21_{and it might be explained by their}

different origins. As described, the crystalline dangling bond
is related to a vacancy complex, which essentially means that
it is characterized by the interplay of electronic effects (due
to impurities) and the local defect geometry. On the other
hand, the amorphous dangling bond is a network defect, which
is consequently essentially influenced by spin delocalization
into the local environment as well as structural features of
*the wider surrounding. Thus the trend for the a parameter*
can be explained by spin delocalization for small strains and
the planar local db structure for large tensile strain. This picture
is also consistent with the trend for the anisotropic hyperfine
*coupling, which shows a gradual increase in p character of the*
db orbital with increasing strain. Overall we learn from this
that for compressive strains delocalization is important and for
tensile strains the db character is enhanced. Most notably, the
latter finding illustrates that spin localizes much more strongly
due to a dangling bond in comparison to regions of strain,
which yield rather delocalized spin distributions.11,12

Let us now discuss the main implication of this conceptual
study for the discrepancy between theory and experiment in the
*a*parameter. Compressive strain on the order of a few percent
can lower the isotropic coupling so that the difference between
both becomes reasonable. However, in this case one should
*also observe a corresponding shift in the b parameter, i.e.,*
the agreement between theory and experiment should become
better as well. Since this is not observed, one cannot consider
strain as an exclusive explanation. But at least it gives a clear
perspective that strain might have an observable influence
on the hyperfine parameters, and consequently may play an
important role for the defect mechanisms in the material.

Furthermore, it points out that an accurate determination
of the anisotropic parameter is decisive for the experimental
analysis and comparison among different samples. For
exam-ple, the current deviation in between [−39, −63] MHz among
different experiments6,7,14 _{can correspond to two opposite}

0.06 0 0.05 0.1
400
350
300
250
200
150
100
*x x0* *x0*
*a*
MH
z
average
*V SiH3*
0.06 0 0.05 0.1
70
60
50
40
30
20
10
*x x0* *x0*
*b*
MH
z

*FIG. 4. (Color online) The dependence of the hyperfine parameters on the elongation x from the ideal lattice constant x*0. For the rhombic

*supercells, x*0*corresponds to the mean lattice constant of the three axis (x*1*, x*2*, x*3). The bond parameters are defined by the average over

the three nearest neighbors. Each thin line corresponds to one db model. The thick blue line indicates the trend for the mean value. Kinks
in this curve can occur when the number of included db models changes with respect to strain. For comparison, the thick dashed line shows
*the dependence of the crystalline V (SiH*3) db model. Values of pressure are included for the experimentally relevant range of strains. The

strain situations. This difference is therefore too large to clearly
*identify the overall contribution of spin delocalization and sp*
hybridization to the defect, which would be important for a
better understanding of the SWE. Our results yield a clear
trend in between spin localization and structural changes due
to strain. Even though the experimentally accessible range of
strain is much smaller as in our study, it would be therefore
interesting to carry out a corresponding experiment.

**IV. CONCLUSIONS**

In this work we have characterized the amorphous Si
dangling bond (db), which was generated from structural
models of a-Si:H by removing one hydrogen atom. This
approach to creating the defect leads to a broad variety of
realizations. We did not impose any constraints or weighting
factors to better reflect the experimentally observed defect
ensemble since we lack sufficient information on the
deci-sive physical mechanisms. Two key characteristics are spin
delocalization and the actual coordination of the db atom.
Only ∼60% correspond to a strongly localized, threefold
coordinated db defect as commonly assumed.5–7 _{However,}

the EPR parameters do not indicate any distinction from the rest of the db ensemble. The mean bond length and bond angle of strongly localized dangling bonds are comparable to their crystalline counterparts, and the rest of the amorphous network. The decisive geometric parameter is the variation in the bond angles, which also makes a reasoning of the hyperfine parameters in terms of the local defect geometry ambitious.

Overall the a-Si:H db corresponds to a network defect, which is generated at suitable geometric distortions in the

network. It differs in this aspect from its crystalline
counter-part, which is usually related to the presence of a vacancy. The
different origins of the c-Si and a-Si:H dangling bond can be
also seen from the systematic study of strain effects on the
hyperfine parameters. Most notably for compressive strains,
*we obtain in the crystalline case an increase of s character*
of the db orbital, whereas for the a-Si:H db delocalization
becomes important.

Our systematic study also shows that strain can have
an important effect on the hyperfine parameters with the
anisotropic coupling being the decisive parameter. This is
particularly interesting since the current variation among
different experiments and samples is rather large.6,7,14 An
experimental investigation of the strain dependence of the EPR
parameters could shed new light into the interplay between
*spin delocalization and sp hybridization of the db orbital,*
which is crucial for the further characterization of the db
defect and the identification of its role in the Staebler-Wronski
effect.

**ACKNOWLEDGMENTS**

This work was supported by the German ministry of Research and Education in the BMBF research project “EPR-Solar” (03SF0328F). Karol Jarolimek and Miro Zeman thank the Dutch Ministry of Economic Affairs for funding, under the EOS-LT program (Project No. EOSLT02028). D.A.D. thanks NSF for support under Grant 09-03225. We are greatly indebted to K. Lips, A. Schnegg, M. Fehr, and G.A. de Wijs for fruitful discussions. Furthermore, we want to thank A. Duff for proofreading the manuscript.

*_{Also: Radboud University, Institute for Molecules and Materials,}

Heyendaalseweg 135, NL-6525 AJ Nijmegen, The Netherlands.

1_{D. L. Staebler and C. R. Wronski,}** _{Appl. Phys. Lett. 31, 292 (1977).}**
2

_{A. Luque and S. Hegedus, Handbook of Photovoltaic Science and}*Engineering (Wiley-VCH, New York, 2003).*

3_{R. A. Street, Hydrogenated Amorphous Silicon (Cambridge}

University Press, Cambridge, 1991).

4_{A. Shah, P. Torres, R. Tscharner, N. Wyrsch, and H. Keppner,}

**Science 285, 692 (1999).**

5_{D. K. Biegelsen and M. Stutzmann,}** _{Phys. Rev. B 33, 3006 (1986).}**
6

_{M. Stutzmann and D. K. Biegelsen,}

**7**

_{Phys. Rev. B 40, 9834 (1989).}_{T. Umeda, S. Yamasaki, J. Isoya, and K. Tanaka,}

_{Phys. Rev. B 59,}4849 (1999).

8** _{A. Kołodziej, Opt. El. Rev. 12(1), 21 (2004).}**
9

_{T. Shimizu,}

_{Jpn. J. Appl. Phys. 43, 3257 (2004).}10_{P. A. Fedders, Y. Fu, and D. A. Drabold,}_{Phys. Rev. Lett. 68, 1888}

(1992).

11_{P. A. Khomyakov, W. Andreoni, N. D. Afify, and A. Curioni,}_{Phys.}

**Rev. Lett. 107, 255502 (2011).**

12_{L. K. Wagner and J. C. Grossman,}_{Phys. Rev. Lett. 101, 265501}

(2008).

13_{J. A. Weil and J. R. Bolton, Electron Paramagetic Resonance}

(Wiley, New York, 2007).

14_{M. Fehr, A. Schnegg, B. Rech, K. Lips, O. Asthakov, F. Finger,}

G. Pfanner, C. Freysoldt, J. Neugebauer, R. Bittl, and C. Teutloff,

**Phys. Rev. B 84, 245203 (2011).**

15_{M. Cook and C. T. White,}** _{Semicond. Sci. Technol. 4, 1012 (1989).}**
16

_{A. H. Edwards and W. B. Fowler,}

**17**

_{Phys. Rev. B 41, 19816 (1990).}_{N. Ishii and T. Shimizu,}

**18**

_{Solid State Commun. 102, 647 (1997).}_{N. Ishii and T. Shimizu,}

**19**

_{J. Non-Cryst. Solids 227, 358 (1998).}_{G. Pfanner, C. Freysoldt, and J. Neugebauer,}

_{Phys. Rev. B 83,}144110 (2011).

20_{P. Johannesen, B. B. Nielsen, and J. R. Byberg,}_{Phys. Rev. B 61,}

4659 (2000).

21_{G. Pfanner, C. Freysoldt, J. Neugebauer, and U. Gerstmann,}_{Phys.}

**Rev. B 85, 195202 (2012).**

22_{G. D. Watkins and J. W. Corbett,}** _{Phys. Rev. 134, A1359 (1964).}**
23

_{B. B. Nielsen, P. Johannesen, P. Stallinga, K. B. Nielsen, and J. R.}

Byberg,**Phys. Rev. Lett. 79, 1507 (1997).**

24_{M. Cook and C. T. White,}_{Phys. Rev. B 38, 9674 (1988).}

25_{A. Stesmans, B. Nouwen, and V. V. Afanas’ev,}_{Phys. Rev. B 58,}

15801 (1998).

26_{A. Stirling, A. Pasquarello, J. C. Charlier, and R. Car,}_{Phys. Rev.}

**Lett. 85, 2773 (2000).**

27_{P. Biswas, D. N. Tafen, F. Inam, B. Cai, and D. A. Drabold,}_{J. Phys.:}

**Condens. Matter 21, 084207 (2009).**

28_{K. Jarolimek, R. A. de Groot, G. A. de Wijs, and M. Zeman,}_{Phys.}

**Rev. B 79, 155206 (2009).**

29_{K. Jarolimek, G. A. de Wijs, R. A. de Groot, and M. Zeman,}_{Phys.}

**Status Solidi A 207, 605 (2010).**

30_{S. Kasap and P. Capper, eds., Springer Handbook of Electronic and}

31_{P. Giannozzi et al.,}** _{J. Phys.: Condens. Matter 21, 395502 (2009).}**
32

_{C. J. Pickard and F. Mauri,}

**33**

_{Phys. Rev. Lett. 88, 086403 (2002).}_{J. P. Perdew, K. Burke, and M. Ernzerhof,}

_{Phys. Rev. Lett. 77, 3865}(1996).

34_{The GIPAW-reconstruction data for the all-electron wave function}

has been generated by Ari P. Seitsonen.

35_{S. Bl¨ugel, H. Akai, R. Zeller, and P. H. Dederichs,}_{Phys. Rev. B 35,}

3271 (1987).

36_{J. M. Spaeth and H. Overhof, Point Defects in Semiconductors and}

*Insulators (Springer, New York, 2003).*

37_{H. J. Monkhorst and J. D. Pack,}** _{Phys. Rev. B 13, 5188 (1976).}**
38

_{C. Freysoldt, G. Pfanner, and J. Neugebauer,}

_{J. Non-Cryst. Solids}

**358, 2063 (2012).**

39_{M. Fehr, A. Schnegg, C. Teutloff, R. Bittl, O. Astakhov, F. Finger,}

B. Rech, and K. Lips,**Phys. Status Solidi A 207, 552 (2010).**

40_{K. Morigaki and H. Hikita,}** _{Phys. Rev. B 76, 085201 (2007).}**
41

_{H. Gleskova, I. C. Cheng, S. Wagner, J. C. Sturm, and Z. Suo,}

_{Solar}

**Energy 80, 687 (2006).**

42_{The db model corresponds to the monovacancy with three of the}